Complex structures, disorder and low dimensionality
-Treatment of oxides and semiconductors by a relativistic
Korringa-Kohn-Rostoker Green function method
Dissertation
zur Erlangung des Doktorgrades der Naturwissenschaften (Dr. rer. nat.)
der
Naturwissenschaftlichen Fakult¨at II Chemie, Physik und Mathematik
der Martin-Luther-Universit¨at Halle-Wittenberg
vorgelegt von
Richard Matthias Geilhufe, M.Sc. geboren am 15.11.1986, in Halle (Saale)
Tag der Verteidigung 17. Dezember 2015
Gutachter:
1 PD Dr. Arthur Ernst, Max-Planck-Institut f¨ur Mikrostrukturphysik 2 Prof. Dr. Steffen Trimper, Martin-Luther-Universit¨at Halle-Wittenberg
Abstract: The thesis describes the implementation of the fully-relativistic Kor-ringa-Kohn-Rostoker Green function method within the full-potential approx-imation. In contrast to previous implementations the single-site scattering problem is obtained by a direct solution of a system of ordinary differential equations. The choice of this approach is motivated from an extensive numerical investigation of the problem. Furthermore, the relativistic KKR method is used to investigate the tuning of band inversion in PbxSn1´xTe alloys. Additionally, a scalar relativistic
approxi-mation was applied to study the low temperature magnetostructure of PrMnO3 and
CaMnO3. With the help of the Mathematica group theory package GTPack single
Ho atoms on a Pt(111) surface are investigated within the framework of crystal field theory.
Zusammenfassung: Diese Arbeit beschreibt die Implementierung einer vollrela-tivistischen Korringa-Kohn-Rostoker-Green-Funktionsmethode in der N¨aher-ung des vollen Zellpotentials. Im Unterschied zu vorhergehenden Implementierun-gen wird die L¨osung des Einzelstreuproblems auf direktem Wege, durch L¨osen eines Systems gew¨ohnlicher Differentialgleichungen gewonnen. Die Wahl dieses Ansatzes wird durch intensive numerische Untersuchungen motiviert. Des weiteren wird die relativistische KKR methode verwendet, um das Anpassen der Bandinversion in PbxSn1´xTe-Legierungen zu untersuchen. Zus¨atzlich wird eine skalarrelativistische
Variante verwendet um die magnetische Struktur von PrMnO3 und CaMnO3 bei
niedrigen Temperaturen zu erforschen. Mit Hilfe des Mathematica Gruppentheorie-Pakets GTPack werden einzelne Ho Atome auf einer Pt (111) Oberfl¨ache im Rahmen der Kristallfeldtheorie untersucht.
Contents
Symbols V
1. Introduction 1
I. Application of non-relativistic methods to complex materials 5 2. The non-relativistic Korringa-Kohn-Rostoker Green function method 7
2.1. The main formalism in a nutshell . . . 7
2.2. The treatment of disorder using the coherent potential approximation 12 2.3. The Heisenberg Hamiltonian and the magnetic force theorem . . . . 13
3. Ab-initio investigation of PrMnO3 and CaMnO3 15 3.1. Why study manganites? . . . 15
3.2. Structure of PrMnO3 and CaMnO3 . . . 17
3.3. Computational methods . . . 18
3.4. Electronic structure . . . 19
3.5. Magnetic structure . . . 22
4. Application of group theoretical methods to magnetic states of Ho on Pt(111) 25 4.1. Introduction . . . 25
4.2. Qualitative discussion . . . 26
4.3. Quantitative discussion . . . 27
4.3.1. Crystal field Hamiltonian . . . 27
4.3.2. Solution of the eigenvalue equation . . . 28
II. Relativistic extension of the Korringa-Kohn-Rostoker Green func-tion method 33 5. Dirac equation and Green function 35 5.1. Dirac equation . . . 35
5.2. Green function . . . 37
II Contents
5.3. Relativistic free space Green function . . . 37
5.4. The Dyson and Lippmann-Schwinger equation . . . 38
6. Relativistic scattering theory 41 6.1. Introduction . . . 41
6.2. The radial Dirac equation for an arbitrary single-site scattering po-tential . . . 42
6.3. Treatment of the non-spherical potential . . . 44
6.3.1. Shape-truncation function . . . 44
6.3.2. The potential matrix . . . 46
6.4. Solution of the free Dirac equation and matching conditions . . . 48
6.5. Numerical solution of the single-site scattering problem . . . 50
6.5.1. Transformation of the differential equations . . . 52
6.5.2. Initial conditions for the regular scattering solution . . . 53
6.5.3. Normalization of regular scattering solutions and single-site t-matrix . . . 55
6.6. Initial conditions for the irregular scattering solution . . . 57
6.7. Implementation . . . 57
6.8. Left-hand side solution . . . 58
6.9. Multiple scattering Green Function . . . 60
6.10. The Lloyd equation . . . 61
III. Tests of the relativistic extension 63 7. The relativistic Coulomb problem 65 7.1. Introduction . . . 65
7.2. Asymptotic behaviour . . . 66
7.3. Exact solution . . . 69
7.4. Numerical accuracy . . . 72
8. The relativistic Mathieu problem 77 8.1. Introduction . . . 77
8.2. Expansion of the Mathieu potential into spherical harmonics . . . 78
8.3. Numerical accuracy . . . 79
8.4. Band structure . . . 82
9. The electronic structure of PbTe and SnTe 85 9.1. Introduction . . . 85
9.2. Crystal structure . . . 85
Contents III
9.4. Electronic structure . . . 86 9.5. Influence of alloying and hydrostatic pressure on band inversion . . . . 88 9.6. Influence of uniaxial strain on band inversion . . . 90
10. Summary 93
IV. Appendix 95
A. Density functional theory 97
B. The Mathematica package GTPack 101
Theses and publications 105
Bibliography 107
Acknowledgements 125
Eidesstattliche Erkl¨arung / Declaration under oath 127
Symbols
The following mathematical symbols are used throughout the text. ˜ A, ˜B, . . . matrices ˆ A, ˆB, . . . operators a, b, . . . vectors A, B, . . . sets i imaginary unit, i2_{“ ´1}
ˆr represents the azimuthal angle ϑ and the polar angle ϕ of the vector r_{“ pr, ϑ, ϕq}
<A real part of A
=A imaginary part of A
Tr ˜A“ ř_{i}Aii denotes the trace of the matrix ˜A
1. Introduction
The Korringa-Kohn-Rostoker Green function method which is applied to cal-culate material properties in the solid state has had a long tradition going back to the early work of Korringa [1] as well as Kohn and Rostoker [2] in 1947 and 1954, respectively. The technological demand for functional materials as well as the de-scription of new physical effects during the past decades offered challenging problems and lead to still ongoing extensions of the original band structure method [3]. Two very prominent extensions are: first, the inclusion of spin-orbit coupling, achieved by solving the Dirac equation instead of the Schr¨odinger equation [4, 5, 6] and, sec-ond, the consideration of the non-spherical part of the crystal field and the shape of the Wigner-Seitz cell at each atomic position, which is denoted as the full-potential approach within the literature [7, 8].
The discussion of spin-orbit coupling in semiconductor physics has a long tradi-tion [9, 10]. However, especially on surfaces spin-orbit coupling driven effects gave new perspectives to solid-state physics during the past 20 years. Examples are the investigation of the Rashba-splitting on metallic surfaces [11, 12] and the descrip-tion of topological insulators [13, 14, 15, 16]. Spin-orbit coupling is propordescrip-tional to the gradient of the electrostatic potential. Therefore, it becomes prominent if heavy elements are taken into account.
The full-potential approach is necessary for the study of elastic properties [17], for the relaxation of crystal structures [18], and especially for the study of systems with large crystallographic anisotropy, as it occurs again on surfaces and interfaces. The investigation of surfaces and interfaces of oxides has become very important in Halle, due to the collaborative research centre SFB 762: Functionality of Oxide Interfaces. Oxides represent a large class of materials, which can be tuned to offer certain electric and magnetic properties with high technological relevance. One example is provided by zinc oxide which can be forced to become a semiconducting ferromagnet by introducing impurities or vacancies [19, 20].
The computer code Hutsepot [21, 22], which is based on the KKR method, has been used successfully for the investigation of oxides and their magnetic properties [23, 24], the treatment of strongly correlated electrons [25, 26] and magnetic excita-tions [27, 28, 29] during the past years. Up to now, a fully-relativistic full-potential implementation of the KKR method like used in other codes [30, 31] was still missing, but has been developed during the work of this thesis.
However, before one can start the discussion of relativistic extensions, results
2 1. Introduction
tained by the non-relativistic KKR method are presented in Part I. Following a short introduction of the non-relativistic KKR method in Chapter 2, a theoretical investigation of the electronic and magnetic structure of PrMnO3 and CaMnO3 is
presented in Chapter 3. Due to their complex structure and their sensitive response to structural or magnetic perturbations, the study of manganites is very challeng-ing and has attracted the attention of the research community durchalleng-ing the past two decades [32, pp. 2-4]. In addition to the relativistic KKR method, a Mathematica [33] group theory package GTPack has been developed, which will be published in a book in the near future [Ge1]. According to an experimental observation, where it was found that magnetic moments of single holmium atoms on a highly conductive metallic substrate can reach lifetimes of the order of minutes [Ge6], the application of group theoretical methods in terms of crystal field theory to such problems is presented in Chapter 4.
In Part II of the thesis an implementation of the fully-relativistic full-potential KKR method for the code Hutsepot will be discussed. The central point of the im-plementation is the solution of the single-site scattering problem. After the successful implementation of a non-relativistic full-potential method of Drittler [7], where this part was solved using the Lippmann-Schwinger equation, it was shown by Huhne et al. [30] that the same approach can also be used to solve the Dirac equa-tion for a non-spherical scattering potential. For the non-relativistic full-potential problem, Zabloudil et al. [34, p. 76] compared the solution by means of the Lippmann-Schwinger equation with the direct solution of the differential equations and illustrated that large deviations between both solutions were found. However, a multitude of efficient and highly accurate numerical methods for the solution of coupled ordinary differential equations with various underlying properties has been developed during the past century [35]. Therefore, in contrast to previous imple-mentations [7, 30], a solver based on the direct solution of the underlying differential equations was developed.
After the theory has been explained in Part II, tests of the implementation [Ge2] are discussed in Part III. For spherically symmetric screened atomic potentials, it was found that the asymptotic behaviour of the irregular scattering solutions in the non-relativistic limit c_{Ñ 8 does not fit to the expected asymptotic behavior of the} non-relativistic irregular scattering solutions close to the origin r ! 1. To under-stand this phenomenon a complete discussion of the Coulomb problem for irregular scattering solutions in Chapter 7 and a proof of the correctness of this behavior by using an elegant transformation of the Dirac equation for spherically symmetric potentials, as suggested by Swainson and Drake [36], will be given. Afterwards the numerical solution of the fully-relativistic single-site scattering problem for the non-spherical Mathieu-potential will be discussed in Chapter 8 by means of inte-gral and differential equations. Since the spherically symmetric component of the Mathieu-potential is in the same order of magnitude as the non-spherical
compo-3
nents it can be seen, first, as a test of the implementation for highly anisotropic potentials and, second, as a good approximation for empty spheres as they are re-quired in the application of the KKR method to oxides. It will be shown that the underlying differential equations are non-stiff and can be solved by applying the Adams-Bashforth-Moulton predictor-corrector method [34, pp. 60-61].
Finally, in Chapter 9 fully-relativistic band structure calculations for the investi-gation of tin and lead telluride alloys SnxPb1´xTe will be presented. Such materials
played a significant role during the 1960s and 1970s [37] as infrared sensors. However, tellurides attracted attention a second time, since they are prominent candidates for the realization of topological insulators [38, 39]. For instance for SnTe, the reason for that is an inversion of the band characteristic at the L-point in the Brillouin zone. It is shown that besides the size of the band gap, also the band inversion can be tuned by alloying, by applying hydrostatic pressure or by applying uniaxial strain.
Part I.
Application of non-relativistic
methods to complex materials
2. The non-relativistic
Korringa-Kohn-Rostoker Green
function method
2.1. The main formalism in a nutshell
Within this section a basic overview about the non-relativistic Korringa-Kohn-Rostoker Green function method is given. The description is shortened as much as possible since a lot of principles are similar to the relativistic version which will be explained in detail in Part II. More detailed descriptions of the non-relativistic KKR method can be found within the literature [7, 40, 41, 42].
The reformulation of the original KKR band structure method [1] in terms of a Green function method [2] has a lot of advantages. For example, the Green function allows the analytical treatment of perturbations (see Section 5.4). Further-more, physical quantities like the charge density and the magnetization density can be calculated if the Green function of a system is known. The formalism can be embedded into the framework of density functional theory (see Appendix A), where the ground state properties of the many particle system can be calculated from the electron density. The electron density is not calculated by solving a many particle Schr¨odinger equation (or Dirac equation) but self-consistently by the solution of an effective one particle Kohn-Sham equation.
The approach via multiple-scattering theory is based on the decomposition of a perfect crystal into distinct scattering centres [3]. Considering a perfect crystal, concentrating on one single atom and substituting all other atoms with vacuum at each lattice site, it is possible to think about a single-site scattering problem, where an initial plane wave excites a spherical wave at the atomic site (see Figure 2.1). Imagine that it is possible to construct the Wigner-Seitz cell Ω around the atom and to define the effective potential Vprq such that it is non-zero in the inside and zero in the outside of the cell. Due to the influence of the neighbouring atoms and the non-spherical shape, the effective potential at each atomic site is non-spherical in general. By using atomic Rydberg units, the Kohn-Sham equation at each site can be formulated as follows
`
´∇2_{` V prq ´ E˘ ψ}
lmprq “ 0. (2.1)
8 2. The non-relativistic Korringa-Kohn-Rostoker Green function method
Figure 2.1.: Illustration of a single-site scattering event.
According to Drittler [7, p. 17], by transforming to spherical polar coordinates and by expanding the effective potential Vprq and the wave function ψlmprq into
spherical harmonics, ψlmprq “ ÿ l1_{m}1 1 rφl1m1,lmprqY m l pˆrq, (2.2)
equation (2.1) can be reformulated in the following way,
ÿ l2 l2 ÿ m“´l2 „ˆ ´_{dr}d2 ` lpl ` 1q r2 ´ E ˙ δll2δ_{mm}2` V_{lm,l}2_{m}2prq φl2_{m}2_{,l}1_{m}1 “ 0. (2.3)
Here, the orthogonality relation of the spherical harmonics was used and Vlm,l2_{m}2prq
denotes the matrix element
Vlm,l2_{m}2prq “
ż
dˆrY_{l}mpˆrq˚_{Y}m2
l2 pˆrqV prq. (2.4)
Whereas equation (2.1) is a partial differential equation in three coordinates, equa-tion (2.3) is an infinitely large system of coupled ordinary differential equaequa-tions. From equation (2.1) it is possible to obtain two linear independent solutions ψ1
lmprq and
ψ2
lmprq, which are called regular and irregular scattering solution, respectively. In
the following ψ1
lmprq and ψlm2 prq will be denoted by Rlmprq and Hlmprq.
Since the potential is zero outside of the Wigner-Seitz cell, the solution of (2.3) in this region is given by a linear combination of the spherical Bessel func-tion _{J}lmprq “ jlp
?
Er_{qY}m
l pˆrq and the spherical Hankel function of the first kind
Hlmprq “ hlp
?
ErqYm
l pˆrq. In general, inside of the Wigner-Seitz cell the regular
and irregular solutions have to be found numerically, where the boundary conditions are given by matching conditions with the free regular and irregular solutions at the
2.1. The main formalism in a nutshell 9
boundary of the Wigner-Seitz cell Ω [7, pp. 18-23], RlmprBq “ JlmprBq ´ i ? E ÿ l1_{m}1 Hl1_{m}1pr_{B}qt_{l}1_{m}1_{,lm}. (2.5) and HlmprBq “ HlmprBq, rBP Ω. (2.6)
In the above equation, tl1_{m}1_{,lm} denote a matrix element of the single-site t-matrix.
For a spherically symmetric potential, the single-site scattering t-matrix is a diagonal matrix tlm,l1_{m}1 “ δ_{ll}1δ_{mm}1t_{lm} and can be related to the phase shift η_{lm} [43, p. 36] via
tlm“ ´
1 ?
Esinpηlmq exp piηlmq . (2.7)
The phase shift ηlm quantifies the shift between a free solution and a scattering
solution for a spatially bounded scattering potential (see Figure 2.2).
In contrast to the single-site scattering event, which was discussed so far, Figure 2.3 illustrates a multiple scattering event, where an initial wave excites several spherical waves at distinct scattering centres along all possible paths. With the help of the single-site solutions Ri
lmprq and Hlmi prq at certain scattering sites i it is possible to
construct the retarded multiple-scattering Green function [44] according to G_{pr ` R}i, r1` Rj, zq “ ÿ lm ÿ l1_{m}1 Ri_{lm}_{pr, zqG}ij_{lml}1_{m}1pzqR j lmpr 1_{, z}_{q`} ` δij ÿ lm Ri_{lm}pră, zqH_{lm}j prą, zq, rP Ωi, r1P Ωj. (2.8) phase shift _{k}η Free solution Scattering solution Potential Radius r |Ψ( r)) | 2 ,V (r ) RBS
Figure 2.2.: Illustration of the phase shift η, describing the shift between a scattering solution outside of a spatially bounded scattering potential and a free solution.
10 2. The non-relativistic Korringa-Kohn-Rostoker Green function method
Figure 2.3.: Illustration of a multiple scattering event along a certain path.
Here, z denotes the complex energy z“ E `iδ and răand rąare an abbreviation for
the one vector of r and r1_{with the smaller and the larger absolute value, respectively.}
Whereas the second term on the right hand side of equation (2.8) represents the single-site scattering contribution of a certain site i, the first one combines regular scattering solutions of the sites i and j and hence represents the multiple-scattering contribution. ˜G_{“}!Gij_{lml}1_{m}1
)
is called structural Green function matrix. Combining all single-site t-matrices of N scattering sites to a matrix ˜T ,
˜ T “ ¨ ˚ ˝ ˜ t1 _{. . .} _{˜}_{0} .. . . .. ˜0 ˜ 0 ˜0 ˜tN ˛ ‹ ‚, (2.9)
the structural Green function matrix can be obtained self-consistently by means of ˜
T and the structure constants ˜G0 _{via the algebraic Dyson equation}
˜
G“ ˜G0` ˜G0T ˜˜G0` ˜G0T ˜˜G0T ˜˜G0` ¨ ¨ ¨ “ ˜G0” ˜I´ ˜T ˜G0 ı´1
. (2.10)
The analytic form of the structure constants can be found i.e. in the book of Zabloudil et al. [34, pp. 24-25]. The convergence of the KKR method can be improved by using so-called screened structure constants, which are discussed in the work of Zeller et al. [44] and Szunyogh et al. [45].
If the Green function is known, it is possible to calculate the density of states as well as the charge density from the imaginary part of the retarded Green function,
npEq “ ´1 π= ż dr Gpr, r, E ` iδq and ρprq “ ´1 π= ż " dz Gpr, r, zq. (2.11)
2.1. The main formalism in a nutshell 11
Instead of calculating the band structure directly, which might be very cumbersome, it is possible to obtain the so called Bloch spectral function via Fourier transfor-mation of the Green function for periodic systems. The imaginary part of the k resolved Green function gives a band structure like result [46, p. 128],
ABpk, W q “ ´ 1 π Im Tr » – ÿ RjPL eik¨Rj ż d3_{r} jGprj, rj` Rj, Wq fi fl. (2.12)
The summation in the last expression extends over all vectors Rj of the lattice
denoted byL. In the framework of density functional theory the charge density can be used to construct a new effective potential and, furthermore, to calculate the total energy of the electron gas [47, p. 61] via
Erρprqs “ Tsrρprqs `
ż
drVprqρprq ` VHrρprqs ` Excrρprqs. (2.13)
Here, Ts denotes the functional for the kinetic energy, VH denotes the Hartree
functional, which takes into account the electron-electron interaction, and last but not least Exc denotes the exchange-correlation functional.
Kohn-Sham equation (2.3)
Scattering solutions and t-matrix for each site
Structural Green function (2.10)
Green function (2.8)
charge density (2.11)
total energy and new effective potential (2.13)
12 2. The non-relativistic Korringa-Kohn-Rostoker Green function method
Whereas in the many particle Schr¨odinger equation the potential is known explicitly, the effective potential of the one-particle Kohn-Sham equation is not. In practice, this effective potential is obtained self-consistently by starting with a trial potential. For the trial potential, it is possible to solve the differential equation (2.3) and to construct the Green function according to (2.8). Afterwards the charge density can be calculated from equation (2.11). In turn, the charge density can be used to calculate the total energy and a new trial potential. This scheme is repeated, until the change of the total energy between two cycles becomes reasonably small. An illustration of the self-consitency cycle of the KKR method can be found in Figure 2.4.
2.2. The treatment of disorder using the coherent potential
approximation
The possibility of alloying materials allows to design technologically relevant prop-erties. For example, the alloy GaAsxP1´x is widely used in optoelectronics for the
fabrication of light emitting diodes (LEDs). The colour of the emitted light varies with increasing amount x of arsenic from red to yellow [48, 49]. The colour of the LED, which is determined by the size of the band gap can be tuned even more by adding a fourth component, as it is possible in GayIn1´yAsxP1´x [50]. Here, a second
concentration y occurs.
For the computation of such materials it is necessary to apply techniques which allow a proper treatment of chemical disorder. A straightforward way is given by constructing large super cells, substituting certain atoms and averaging the possible configurations. Even though this procedure was already applied successfully [51] it has the disadvantage that it is restricted to concentrations that can be represented by stoichiometric compounds. The development of mean field theories opened a second approach to the problem. Regarding a binary alloy AxB1´x, the simplest
approxi-mation for an electronic structure calculation is the introduction of an hypothetical element with the average potential Vprq “ xVAprq ` p1 ´ xqVBprq, which is denoted
as the virtual crystal approximation [52, 53].
A more reliable Green function method was suggested by Soven in 1967 [54], which is called the single-site coherent potential approximation (CPA). A somehow similar approach was communicated by Velick´y, Kirkpatrick and Ehrenreich in 1968 [55]. In both approaches an effective mean field medium is introduced. Later, the method was simplified by Gyorffy [56]. Considering an alloy with N components, where each component has the concentration xi and the sum over all concentrations
is restricted by ř
ixi “ 1. It is hypothesised that the total scattering of electrons
2.3. The Heisenberg Hamiltonian and the magnetic force theorem 13
scattering at averaged atoms within the effective medium,
N ÿ i“1 xiτ˜i,nn 1 pEq “ ˜τnn1 CPApEq. (2.14)
Here, the scattering path operator ˜τ is introduced, which is given by ˜
τnn1pEq “ δnn1˜tnpEq `
ÿ
m‰n
˜
tnpEqG0,npEq˜τmn1pEq. (2.15) The single site scattering t-matrix ˜tn
CPA of the CPA medium at a certain site n is
defined implicitly from the scattering path operator ˜τnn1
CPA via equation (2.15) and
has to be found self-consistently by starting with a reasonable trial matrix ˜tn,0_{CPA} [3]. Solving the single-site scattering problem for each component and using the com-ponent projected scattering matrix ˜τi,nn1
to construct the multiple scattering Green function Gi_{pr, r}1_{, E}_{q, the averaged Green function of the effective medium can be}
approximated by summation [57, 3], Gpr, r1_{, E}_{q “} N ÿ i“1 xiGipr, r1, Eq. (2.16)
The coherent potential approximation is implemented within Hutsepot and will be used later on during this thesis, e.g. in Chapter 9.
2.3. The Heisenberg Hamiltonian and the magnetic force
theorem
In collinear magnetic systems (ferromagnetic, antiferromagnetic or ferrimagnetic) the magnetic moments of the atoms within a crystal are either parallel or anti-parallel to the global magnetization axis. Presuming the existence of permanent, localized moments interacting with each other via a direct or an indirect exchange mechanism, it is possible to formulate a semi-classical effective many particle Hamiltonian, called the Heisenberg Hamiltonian [58],
ˆ
Heff_{“ ´}ÿ
i,j
Jijei¨ ej. (2.17)
Here, the vectors eidenote the unit vectors pointing into the direction of the spins Si.
The name refers to the early work about the theory of ferromagnetism by Heisen-berg in 1928 [59]. Since the equilibrium magnetic ordering can be found by minimiz-ing the energy of the Heisenberg Hamiltonian, the magnetic moments of the atoms tend towards a parallel alignment (ferromagnetism) for exchange parameters Jij ą 0
14 2. The non-relativistic Korringa-Kohn-Rostoker Green function method
and towards an anti-parallel alignment (antiferromagnetism) for exchange parame-ters Jij ă 0. Especially for the description of magnetic insulators the Heisenberg
model can be applied successfully [60]. For the relativistic case, the Heisenberg model can be extended and additional terms like the Dzyaloshinskii-Moriya in-teraction [61, 62, 63] occur.
The Heisenberg exchange parameters Jij can be calculated via the magnetic
force theorem and the approach of Liechtenstein et al. [64], where the exchange parameters are determined from the rotation energy of two spin moments at sites i and j on opposite angles ˘θ{2,
δEij “ p1 ´ cos θq «
1 2Jijθ
2_{.} _{(2.18)}
With the help of the Lloyds formula (see Section 6.10) the energy difference is expressed using the single-site scattering t-matrices ˜tiσat site i for the spin direction
σ as well as the scattering path operator ˜τij _{(see equation (2.15)). Then the exchange}
parameters Jij are calculated by means of the following equation [64, 3],
Jij “ ´ 1 4π= żEF ´8 dE Tr”´˜t´1 iÒ ´ ˜t ´1 iÓ ¯ ˜ τ_{Ò}ij´˜t´1 jÒ ´ ˜t ´1 jÓ ¯ ˜ τ_{Ó}jiı. (2.19)
The above presented concepts of this chapter are applied to the investigation of PrMnO3 and CaMnO3 within the next chapter.
3. Ab-initio investigation of PrMnO
3
and
CaMnO
3
3.1. Why study manganites?
During the past two decades the study of manganites has become more and more prominent within the condensed matter community. For the increasing interest at least three reasons can be emphasized [32, pp. 2-4]. First, manganites tend to show “colossal magnetoresistance”, where the resistivity increases by many orders of magnitude upon the application of small magnetic fields. Materials with notable magnetotransport properties are technologically relevant for instance in the develop-ment of hard disk drives with large storage capacity [65]. Second, some manganites are intrinsically inhomogeneous with coexisting clusters of different phases, mostly ferromagnetic and antiferromagnetic clusters. As an example, Svedberg et al. [66] found coexisting spin-glass and ferromagnetic phases for Pr0.9Ca0.1MnO3 thin films
at low temperatures. Third, manganites show rich phase diagrams with unusual spin, charge, lattice, and orbital order. Phase diagrams of manganites were dis-cussed by Tokura and Tomioka [67]. An illustration for Pr1´xCaxMnO3 alloys
with a calcium content between 0% and 50% can be found in Figure 3.1. Whereas Pr1´xCaxMnO3 remains insulating within the whole range, the magnetic ordering
changes a lot. Starting from an A-type antiferromagnetic structure for x_{“ 0, where} a ferromagnetic inter-plane and an antiferromagnetic intra-plane coupling of man-ganese atoms is present, manman-ganese moments are slightly canted for low concen-trations xă 0.15, which is denoted as the spin-canted insulating phase (CI). Then, between x_{“ 0.15 and x “ 0.3 a ferromagnetic phase (FI) is observed for low } tempera-tures. In the range of x“ 0.3, . . . , 0.5 the material becomes antiferromagnetic again, with successive magnetic transitions between an antiferromagnetic phase (AFI) and a canted antiferromagnetic phase (CAFI).
A theoretical study of manganites is challenging as can be verified within the literature [68, 69]. Again three main reasons can be pointed out. First, driven by the fact that manganites are intrinsically inhomogeneous one needs a microscopic description to understand the mechanisms behind a certain phase combined with a mesoscopic method to understand their interplay. Second, by focusing on the microscopic description, density functional theory based methods are facing problems caused by highly localized d and f electrons leading to strong correlations [70, 71]. To
16 3. Ab-initio investigation of PrMnO3 and CaMnO3
achieve reasonable results one can either improve the exchange correlation functional by climbing up the “Jacob’s ladder of density functional approximations” [72] to generalized gradient approximations or higher or by applying explicit correlation corrections like the self-interaction correction [73, 25] or the so-called Hubbard-U method [74]. Third, if one is interested in the description of phase diagrams one needs to take into account temperature. On the one hand ground state calculations can be extended by smoothening the occupation of states by means of the Fermi-Dirac distribution function [75] or by mean-field methods like the disordered local moment method [76, 77]. On the other hand dynamical excitations like lattice vibrations have to be taken into account where the resulting electron-phonon coupling has to be included [78]. 0.1 0.2 0.3 0.4 0.5 0 50 100 150 200 250 300 PI COI AFI CAFI FI CI TN TC TN TCO TCA Ca content x T emp eratur e (K)
Figure 3.1.: Phase diagram of Pr1´xCaxMnO3 (illustration adopted from [67]). The
abbreviations denote paramagnetic insulator (PI), ferromagnetic insu-lator (FI), antiferromagnetic insuinsu-lator (AI), spin-canted insuinsu-lator (CI), charge-ordered insulator (COI), and canted-antiferromagnetic insulator (CAFI).
3.2. Structure of PrMnO3 and CaMnO3 17
(a) Real space elementary cell
kx kz ky Z U X S Y T Γ R (b) Brillouin zone
Figure 3.2.: Real space orthorhombic crystal structure and Brillouin zone with high symmetry points of PrMnO3 and CaMnO3. In the picture of the
real space elementary cell oxygen atoms are illustrated in red and man-ganese atoms in purple. Yellow atoms are representing praseodymium and calcium, respectively [80].
3.2. Structure of PrMnO
_{3}and CaMnO
_{3}The manganites PrMnO3 and CaMnO3 are crystalizing in an orthorhombic crystal
structure with the space groups pbnm and pnma. Both space groups share the same space group index 62. The real-space structure of both materials is illustrated in Figure 3.2a. The Brillouin zone of the orthorhombic unit cell is shown in Figure 3.2b. A summary of the lattice constants and atomic positions that where used during the calculations can be found in Table 3.1.
As can be verified in Figure 3.2a, the manganese atoms are surrounded by six oxygen atoms forming a slightly distorted octahedron. Each praseodymium and calcium atom is surrounded by eight of such octahedra, which are canted into the crystallographic a and b direction. For a perfect octahedron the manganese d states would split into a threefold degenerate state T2g and a twofold degenerate state Eg,
as can be verified with the help of the Mathematica group theory package GTPack [Ge4]. However, for PrMnO3 and CaMnO3 it is favoured to decrease the symmetry
furthermore leading to a splitting of the T2g and Eg states into states with lower
degeneracy [32, pp. 57-69]. As a result the occupied levels are lower in energy and hence also the total energy of the system is decreased. This phenomenon, which is known as Jahn-Teller distortion, was initially described by Jahn and Teller in 1937 [79].
18 3. Ab-initio investigation of PrMnO3 and CaMnO3 Cell (PrMnO3) Space group PBNM (62) Lattice constants [˚A] 5.5326(2) 5.6176(2) 7.8513(3) Angles 90.00000 90.00000 90.00000 Wyckoff positions Pr (4c) 0.992(1) 0.0350(8) 0.250 Mn (4b) 0.5 0 0 O (4c) 0.0762(7) 0.4825(7) 0.250 O (8d) 0.7126(5) 0.2970(4) 0.0416(3) Cell (CaMnO3)
Space group PNMA (62)
Lattice constants [˚A] 5.28930 7.45644 5.27074 Angles 90.00000 90.00000 90.00000 Wyckoff positions Ca (4c) 0.0198(17) 0.25000 -0.004(4) Mn (4b) 0.00000 0.00000 0.50000 O (4c) 0.493(2) 0.25000 0.0658(20) O (8d) 0.2882(10) 0.0362(9) -0.2917(10)
Table 3.1.: Experimental structure data of PrMnO3 [81] and CaMnO3[82]. The data
was used for the construction of the unit cell for the calculations.
3.3. Computational methods
The following results were obtained from calculations using a screened scalar-rela-tivistic Korringa-Kohn-Rostocker Green function method [83, 84], as imple-mented in Hutsepot [21]. The electron density was calculated by means of a multipole expansion, taking into account the shape of the Voronoi polyhedra around each atom within the unit cell [85, 86]. For the integration of the imaginary part of the Green function over the energy to calculate the electron density (see equation (2.11)), a semi-circular energy contour was chosen, consisting of 24 points. The ex-pansion of the Green function into spherical harmonics was restricted to a maximal angular momentum of 3.
The unit cell was constructed according to the data of Table 3.1, where four manganese atoms, four praseodymium or calcium atoms and 12 oxygen atoms are present. To achieve better convergence for the self-consistent calculations, ten ad-ditional empty spheres were added at non-occupied crystallographic sites using the
3.4. Electronic structure 19
Stuttgart TB-LMTO program[87]. Due to the large unit cell a mesh of 8_{ˆ8ˆ4 points} was sufficient for integration in k-space. As an approximation for the exchange-correlation functional the revised generalized gradient approximation PBE-SOL was used [88], as it is implemented within the LibXC database [89]. To treat the strongly correlated electrons the Hubbard-U method (or GGA+U method) was applied to manganese d states and praseodymium f states with values of Ud“ 1 ´ 1.25 eV and
Uf “ 5 eV, respectively. The Heisenberg exchange parameters Jij were calculated
by means of the magnetic force theorem, according to equation (2.19). The obtained exchange parameters were used to calculate the critical temperature by means of a Monte-Carlo method implemented by Fischer [40].
Furthermore, results for PrMnO3with and without relaxation of the unit cell, were
compared to each other. The relaxation of the unit cell was obtained by using the Vi-enna ab initio simulation package (VASP) [90]. Analogously to Sathyanarayana, a Γ centred 6ˆ6ˆ6 k-point mesh was applied [91]. Calculations were done using the high performance mode and a plane wave energy cut-off of 400 eV. The relaxation was restricted to that of the lattice parameters whereas the positions of the atoms and the cell shape were fixed. The minimum was found by using a conjugate-gradient algorithm [92, pp 413-417]. In accordance with the KKR calculations the general-ized gradient approximation was used and a Hubbard-U was applied to manganese d states (1 eV) and praseodymium f states (5 eV). It was found that the unit cell volume decreases slightly, but the general results, such as the density of states or the Heisenberg exchange parameters, are not affected.
3.4. Electronic structure
Both materials, PrMnO3 as well as CaMnO3, are semiconductors with experimental
band gap energies of «0.83 eV [93] and «1.55 eV [94], respectively. Due to correla-tion effects, this property is not reproduced within a calculacorrela-tion using the generalized gradient approximation only. Therefore, the Hubbard-U method was applied. The choice of an appropriate value of U is crucial, since physical quantities like the size of the band gap, the magnetic moment of manganese and praseodymium, the Heisen-berg exchange parameters Jij, the magnetic ordering and the critical temperature
are sensitive to the magnitude of U . For PrMnO3 the Hubbard-U was applied to
praseodymium f -states (Uf) and manganese d-states (Ud). Calculations were
per-formed for Uf = 3, 4, 5, 6 eV and Ud = 0, 1, . . . , 4 eV. The best agreement with
experimental values for the band gap and the critical temperature [95] was achieved for Uf = 5 eV and Ud“ 1 eV.
According to the Bloch spectral function (see Figure 3.3a) it can be verified that PrMnO3 is an indirect semiconductor, where the valence band maximum can be
20 3. Ab-initio investigation of PrMnO3 and CaMnO3
(a) Bloch spectral function
−6 −4 −2 0 2 0 20 40 60 Total DOS Pr f -states Mn d-states Energy (eV) DOS (states/eV/c ell)
(b) Density of states (DOS)
Figure 3.3.: Electronic structure of PrMnO3.
zone. The band gap is slightly underestimated and shows a value of« 0.5 eV which is also reflected in the density of states in Figure 3.3b. From the density of states it can be verified that the valence band maximum as well as the valence band minimum is dominated by manganese d-states. Beyond the Fermi energy two sharp peaks can be seen, which belong to non-occupied praseodymium f -states. The range between -7 eV and -2 eV is dominated by oxygen p-states.
For CaMnO3 the best agreement with experimental values (such as magnetic
mo-ment, band gap, etc.) was obtained for a slightly increased value of Ud “ 1.25 eV.
Analogously to PrMnO3, CaMnO3 is an indirect semiconductor as well, as can be
verified from Figure 3.4a where the valence band maximum is located along the path Y Γ and the conduction band minimum at Γ and Y . Again, the size of the band gap is about 0.5 eV. In contrast to PrMnO3, the manganese d-states are hybridizing
with oxygen p-states for CaMnO3 in the whole range of the valence band between
-6 eV and 0 eV, as can be seen in the density of states illustrated in Figure 3.4b. The conduction band is dominated mainly by manganese d-states.
For PrMnO3 and CaMnO3 a change of the oxidation state of manganese can be
observed. The electron configuration of manganese is given by [Ar] 3d5 _{4s}2_{. Due to}
the two s- and five f -electrons, possible oxidation states for manganese in compounds are between`2 and `7. Since calcium belongs to the group of alkaline earth metals it carries two s-electrons in the outermost shell leading to an oxidation number of `2 in CaMnO3. Together with the oxidation state of ´2 for oxygen, manganese is
forced to have an oxidation state of `4. According to Hund’s rule the remaining d-electrons are occupying different d-orbitals with a parallel spin alignment leading
3.4. Electronic structure 21
(a) Bloch spectral function
−6 −4 −2 0 2 4 0 5 10 15 20 Total DOS Mn d-states Energy (eV) DOS (states/eV/c ell)
(b) Density of states (DOS)
Figure 3.4.: Electronic structure of CaMnO3.
to a magnetic moment of 3 µB. Corresponding to Jir´ak et al. [96], a slightly lower
magnetic moment of 2.66 µB was measured in neutron diffraction experiments.
Nevertheless, this value is in very good agreement to the present calculations, where a magnetic moment of 2.7 µB was observed on each manganese atom. For PrMnO3
the calculated magnetic moment is given by 3.6 µBleading to the conclusion that the
oxidation state of manganese has decreased. Again, the experimental value of 3.54 µB
is in very good agreement [96] with the calculation. Anyway, since the experimental as well as the calculated manganese magnetic moments are non-integer values it is very likely that mixed configurations of manganese`4 and `3 as well as manganese `3 and `2 are present in PrMnO3and CaMnO3, respectively. Regarding the electron
configuration of praseodymium, which is given by [Xe] 4f3 _{6s}2 _{an oxidation state of}
`3 will give a magnetic moment of 2 µB which results from the occupation of two
distinct f -orbitals of the remaining two 4f electrons with parallel spin alignment. In accordance, the computational value for the magnetic moment of praseodymium in PrMnO3 was found to be exactly 2 µB. However, this value stays in contrast to the
experimental value of Jir´ak et al. who suggested a magnetic moment of 0.5 µB [96].
Nevertheless, in recent neutron diffraction experiments [97], the present theoretical prediction of the praseodymium high-spin state 2 µBwas used to fit the experimental
22 3. Ab-initio investigation of PrMnO3 and CaMnO3
results and was found to be more likely than the previous result of Jir´ak et al. [96].
3.5. Magnetic structure
To obtain information about the magnetic structure the magnon spectrum of PrMnO3
and CaMnO3was calculated. Assuming collinear magnets and the adiabatic
approxi-mation, the magnon spectrum can be found from the eigenvalues of the torque matrix [41, pp. 31-34]. According to Figure 3.5a, the minimum of the magnon spectra for PrMnO3 is located at the Z point in the Brillouin zone. Furthermore the spectrum
is symmetric, regarding positive and negative energies. Hence, the magnon spectrum does not show a ferromagnetic behaviour, which is in agreement with the literature [96]. It was suggested by Jirak et al. that PrMnO3 is an A-type antiferromagnet
[96, 69], meaning that the intra-plane coupling is ferromagnetic while the inter-plane coupling is antiferromagnetic. The antiferromagnetic ordering can be verified by re-garding the Heisenberg exchange parameters Jij (see Figure 3.6a). The results of
the calculations show large and positive Heisenberg exchange parameters between manganese atoms within the a-b-plane (J=9.4 meV), which cause the in-plane ferro-magnetic ordering. The coupling between praseodymium and manganese tends to be ferromagnetic (J«1-2 meV). For the magnetic coupling between two manganese planes, positive exchange parameters can be found for the coupling between Mn1 and Mn3 (J=3.8 meV), whereas negative exchange parameters can be observed for the interaction between Mn1 and Mn4 (J=-1.2 meV). Even though the absolute value
Γ Z T Y Γ X S R U −100 −50 0 50 100 Energy (eV) (a) PrMnO3 Γ Z T Y Γ X S R U −20 0 20 Energy (eV) (b) CaMnO3
Figure 3.5.: Magnon spectra of PrMnO3 and CaMnO3 calculated using the torque
3.5. Magnetic structure 23
(a) PrMnO3
(b) CaMnO3
Figure 3.6.: Calculated Heisenberg exchange parameters Jij for PrMnO3 and
CaMnO3. 8ˆ ´1.2 meV for instance denotes that 8 equivalent atoms
and hence 8 equivalent exchange parameters are present.
of -1.2 meV is smaller than 3.8 meV, Mn4 occurs eight times in the neighbourhood of Mn1 whereas Mn3 only occurs 2 times. Furthermore, the calculated Heisen-berg exchange parameters were used to confirm the magnetic ordering by means
24 3. Ab-initio investigation of PrMnO3 and CaMnO3
of a Monte Carlo method (for details of the method see [40, pp. 34-35]), where the antiferromagnetic structure was clearly revealed and a transition temperature of « 120 K could be found. However, the system seems to be at the border between antiferromagnetism and ferromagnetism and therefore it reacts very sensitive with respect to small perturbations.
For CaMnO3, Wollan and Koehler [99] found a G-type antiferromagnetic
ordering using neutron diffraction experiments, where both intra-plane and inter-plane coupling are antiferromagnetic. This type of antiferromagnetic coupling agrees well with the calculated values for the Heisenberg exchange parameters in Figure 3.6b. Since calcium is non-magnetic, the Heisenberg exchange parameters Jij for
CaMnO3only describe coupling between manganese atoms. According to the results,
all parameters are negative and hence both inter- and intra-plane coupling tends to be antiferromagnetic. The calculated critical temperature of 91 K is slightly lower than the experimental critical temperature of 110 K.
4. Application of group theoretical
methods to magnetic states of Ho on
Pt(111)
4.1. Introduction
Within the past decades, the data storage capacity of memory devices has increased rapidly [100]. In magnetic data storage, where ferromagnetic materials are used, this trend has led to a decrease of the size of magnetic islands, in which each bit is stored. To keep their magnetization in a specific direction against thermal fluctuations mate-rials with high magnetic anisotropy are needed. In recent years, magnetic anisotropy
(a) Trigonal neighbourhood of a single Ho atom on Pt (111).
(b) Three-dimensional topographic STM image of single Ho atoms adsorbed on Pt(111) at 4.4 K.
(c) Spin-polarized dI/dV map of Ho atoms and Co islands on Pt(111) (V = 300 mV, I = 1.5 nA). Positions of Pt atomic steps are indi-cated by dashed lines.
Figure 4.1.: Illustration of Ho on a Pt(111) surface. The pictures in (b) and (c) were obtained by Miyamachi et al. using scanning tunneling microscopy [Ge6].
26 4. Application of group theoretical methods to magnetic states of Ho on Pt(111)
measurements were performed using scanning tunnelling microscopy for a wide range of substrates and atoms [101, 102, 103]. A first breakthrough was achieved by the work of Hirjibehedin et al. [104] who discovered a large anisotropy for iron and manganese atoms on a thin layer of copper nitride.
A major reason for unstable magnetic moments on surfaces is seen by the action with scattering electrons. Since f electrons are strongly localized the inter-action of f -electrons and surface electrons is weaker in comparison to systems were the valency electrons are d-electrons. Since f -electrons are causing large magnetic moments in single-atoms, promising candidates for single-bit data storage devises are rare earth atoms. In cooperation with the experimental group of Wulfhekel (at KIT Karlsruhe), magnetic excitations of gadolinium atoms on platinum (111) and copper (111) surfaces [Ge7] as well as holmium atoms on a platinum (111) surface [Ge6] were investigated (see Figure 4.1). Surprisingly it could be observed that the magnetic excitations in single holmium atoms on high conducting surfaces can reach lifetimes of the order of minutes.
Besides a description via ab initio methods, group theoretical methods in the framework of crystal field theory were developed [Ge4] and implemented within the Mathematicagroup theory package GTPack [Ge1]. During this chapter it will be ex-plained, how such methods can be applied to describe the large magnetic anisotropy as well as the long lifetimes of magnetic excitations in single holmium atoms on a platinum (111) surface.
4.2. Qualitative discussion
At first, a qualitative discussion of the level splitting for a single holmium atom on a platinum (111) surface will be given. For the electronic structure of holmium it is assumed that 10 electrons occupy the 4f state [105]. Due to spin orbit coupling the 14-fold degenerate 4f state (spin is taken into account) splits into a 6-fold degenerate state 4f5_{{}2 and an 8-fold degenerate state 4f7_{{}2. Since 4f5_{{}2 is lower in energy [106]
four electrons occupy 4f7_{{}2 which leads to a total angular momentum of J “ 8.
For J _{“ 8 it is possible to construct 17 basis vectors |8mi (m “ ´8, . . . , 8) } belong-ing to the irreducible representation D8_{. Representation matrices of proper rotations}
of D8_{are given by the Wigner-D-matrices of each group element of the group SOp3q}
and can be calculated using Mathematica. For improper rotations a factor_{p´1q}J _{has}
to be multiplied. From the matrix element theorem [107, pp. 130-134] it is known that each irreducible representation leads to an energy level of which the degeneracy is equal to the dimension of the irreducible representation.
For a single holmium atom on a platinum (111) surface the local symmetry is decreased by the crystal field of the surface and the associated point group is given by C3v (see Figure 4.1a). For the point group C3v the representation given by matrices
4.3. Quantitative discussion 27
of D8 _{is reducible. The number of times an irreducible representation occurs within}
a reducible representation can be calculated from
np “ 1 g ÿ T rχp_{pT qs}˚_{χ}_{pT q,} _{(4.1)}
which can be derived from the orthogonality theorem for characters [Ge1]. Here, g is the order of the group and the characters χpT q are given by the trace of the representation matrix of the element T . To calculate the characters of the irreducible representations the Burnside algorithm [108] was implemented in the Mathematica group theory package GTPack. From equation (4.1) it is possible to verify that D8
is reducible according to
D8 „ 3A1‘ 6E ‘ 2A2. (4.2)
In the equation above, the Mulliken notation is used [109, 110], where A1 and A2
are the symmetric and the antisymmetric one-dimensional irreducible representations and E the two-dimensional irreducible representation of C3v. The character table of
C3v can be found in Table 4.1.
C1 C2 C3 A1 1 1 1 A2 1 1 -1 E 2 -1 0 C1 “ tEu C2 “ C3z, C3z´1 ( C3 “ tIC2y, IC2C, IC2Du
Table 4.1.: Character table and classes of the point group C3v, calculated with
GT-Pack_{[Ge1]. Symmetry elements are denoted in Sch¨}onflies notation.
4.3. Quantitative discussion
In connection to the qualitative analysis of the splitting of holmium energy levels in a trigonal crystal field, it will be described in this section how the strength of the splitting can be approximated in the framework of linear perturbation theory. First, it will be explained how the crystal field Hamiltonian can be achieved if the point group is known and second it will be shown how the eigenvalue equation can be solved in an efficient way.
4.3.1. Crystal field Hamiltonian
In the following, it is assumed that the solution of a reference Hamiltonian ˆH0 is
known and the influence of the crystal field is small enough to treat it as a pertur-bation. The Hamiltonian of the perturbed system is given by ˆH _{“ ˆ}H0` Vcr. The
28 4. Application of group theoretical methods to magnetic states of Ho on Pt(111)
crystal field can be expanded into tesseral harmonics (real spherical harmonics) S_{k}q,
Vcrpθ, φq “ 8 ÿ k“0 k ÿ q“´k B_{k}qS_{k}qpθ, φq, (4.3)
where the radial part of the crystal field is included in the coefficients B_{k}q. The crystal field has a certain symmetry reflected in the point groupG. Since the Hamiltonian is an irreducible tensor operator belonging to the identity representation Γ1 of G, it
has to be invariant under the application of the character projection operator ˆ_{P}Γ1_{,}
ˆ PΓ1_{V} crpθ, φq “ 1 g ÿ T PG ˆ P_{pT qV}crpθ, φq “ Vcrpθ, φq. (4.4)
The tesseral harmonics Sq_{k}are a real space representation of thep2k `1q-dimensional basis belonging to the irreducible representation Dk_{. Hence, every transformation}
can be expressed via ˆPpT qS_{k}q “ řk_{q}1_{“´k}D_{q}k1_{q}pT qS
q1
k. Using the expansion of the
crystal field (4.3) together with (4.4) it is possible to obtain a system of equations for B_{k}q by comparison of coefficients,
Bq_{k}“ 1 g ÿ T PG ÿ q1 B_{k}q1Dk_{q}1_{q}pT q. (4.5)
Of course, (4.5) can not be solved for all B_{k}q but it can be verified which coefficients depend on each other and which coefficients vanish. For the point group C3v, which
is the point group of the crystal field of a single holmium atom on a platinum (111) surface, the crystal field expansion is given by
Vcrpθ, φq “ B00S00pθ, φq ` B20S20pθ, φq ` B40S40pθ, φq`
` B3
4S43pθ, φq ` B60S60pθ, φq ` B63S63pθ, φq ` B66S66pθ, φq ` . . . . (4.6)
In the following it will be shown, how the crystal field expansion can be used to calculate the level splitting explicitly.
4.3.2. Solution of the eigenvalue equation
In the linear perturbation theory [111, pp. 203-207], the energy difference of the perturbed and the unperturbed system can be calculated from the eigenvalues of the matrix ˜A with elements
Amm1 “ hJm| V_{cr}
ˇ
ˇJm1 . (4.7)
It was the idea of Stevens [112] to generalize the crystal field expansion (4.3) and to replace the tesseral harmonics S_{k}qby associated operators ˆO_{k}qacting on the vectors
4.3. Quantitative discussion 29
|Jmi. The operators ˆOq_{k} can be expressed in terms of ˆJz and the ladder operators
ˆ
J` and ˆJ´, where the well known equations
ˆ
Jz|Jmi “ m |Jmi , and ˆJ˘|Jmi “apJ ¯ mqpJ ˘ m ` 1q |Jm ˘ 1i (4.8)
hold. Tables of the operators ˆO_{k}q can be found in the literature, e.g. [113]. Instead of applying the operators ˆOq_{k}, it was proposed by Ryabov [114] to directly calculate the matrix elements_{hJm| ˆ}O_{k}q_{|Jm}1_{i using the equation}
hJm| ˆOq_{k}ˇˇJm1 “ _{2F}α k,q k´q ÿ n“0 ˜ δm1_{,m`q} „ pJ ´ mq!pJ ` m ` qq! pJ ` mq!pJ ´ m ´ qq! 1_{{}2 ` `δm1_{,m´q}p´1qk´q´n „ pJ ` mq!pJ ´ m ` qq! pJ ´ mq!pJ ` m ´ qq! 1_{{}2¸ mnapk, q, nq. (4.9) Here, Fk,q is given by the greatest common divisor of the coefficients apk, q, 0q, . . . ,
apk, q, qq. Furthermore, α “ 1 for all q if k is an odd integer. If k is even, then α “ 1 or α _{“} 1{_{2} _{for even and odd q, respectively. In case that q}` n ą k all coefficients
apk, q, nq are equal to zero. For q “ k they are apk, k, 0q “ 1. The values of apk, q, nq have to be calculated recursively by
apk, q ´ 1, nq “ p2q ` n ´ 1qapk, q, n ´ 1q ` „ qpq ´ 1q ´mpm ` 1q 2 apk, q, nq` ` k´q´n ÿ ν“1 p´1qν „ˆ n_{` ν} n ˙ JpJ ` 1q ´ ˆ n_{` ν} n´ 1 ˙ ´ ˆ n_{` ν} n´ 2 ˙ apk, q, n ` νq. (4.10) For the application of Ryabovs method three major advances can be pointed out. First, an exact representation of|Jmi is used and hence, the method can be applied easily for many electron systems. Second, in comparison to the classical method, no integration of wave functions is needed and hence, the method is much faster for large J. Third, the equations are exact and can be evaluated algebraically. Using (4.9) thep2J ` 1q dimensional matrix of the Hamiltonian can be calculated via
Hmm1 “ 2J ÿ k“0 k ÿ q“´k Bq_{k}hJm| ˆO_{k}qˇˇJm1 . (4.11)
For a single holmium atom on platinum (111), the values of B_{k}q were calculated from first principles by means of Hutsepot and can be found in Table 4.2. Details of the method are explained within the thesis of Hoffmann [115]. Since J “ 8 the Hamiltonian is represented by a 17_{ˆ17 matrix. The eigenvalues and eigenvectors can}
30 4. Application of group theoretical methods to magnetic states of Ho on Pt(111) coefficients value B0 2 -239 µeV B0 4 86 neV B3 4 293 neV B0 6 0.187 neV B3 6 -1.968 neV B6 6 0.630 neV
Table 4.2.: Crystal field parameters for a single holmium atom on a platinum (111) surface [Ge6, suppl. inf.].
be found using Mathematica. From the eigenvectors ai _{(i} _{“ 1, . . . , 17) it is possible}
calculate the expectation value _{hJ}zi via
hJzi “ 2J `1 ÿ m“1 ˇ ˇai_{m} ˇ ˇ 2 hJm| ˆJz|Jmi . (4.12)
According to Figure 4.2, a large level splitting of « 44.76 meV can be observed. By assigning the energy eigenvalues as well as the basis functions to a certain irreducible representation of C3v, the prediction (4.1) can be confirmed. The ground state
belongs to the irreducible representation E offering two states with hJzi « `8 and
hJzi « ´8, respectively.
To discuss the transition probability, the time-reversal operator ˆT can be taken into account, which commutes with the Hamiltonian ˆH, since no external magnetic field is applied. Moreover, it anti-commutes with the components of the angular momentum operator
ˆ
H ˆT ´ ˆT ˆH “ 0 and ˆJiTˆ` ˆT ˆJi “ 0. (4.13)
The time-reversal operator is an anti-unitary operator, i.e.
hφ|ψi “D ˆT ψ| ˆT φE“D ˆT φ| ˆT ψE˚. (4.14) Furthermore, an even number of electrons is discussed and it follows that ˆT2 _{“ ˆ1.}
Denoting the two degenerate ground-states by|Ψ8i and |Ψ´8i, it can be verified that
hΨ8| ˆJi|Ψ´8i “ ´D ˆT Ψ8 ˇ ˇ ˇJˆiTˆ|Ψ´8i ˚_{“ ´ hΨ} 8| ˆJi|Ψ´8i˚“ ´ hΨ´8| ˆJi|Ψ8i . (4.15)
Hence, hΨ8| ˆJi|Ψ´8i “ 0 and a direct transition between the two ground states is
forbidden. Since a direct transition is forbidden, it follows that under real conditions, where T _{ą 0 K, a long lifetime for staying in one of the two states |Ψ}´8i or |Ψ8i
4.3. Quantitative discussion 31 E (meV) _{hJ}zi Γ 0. 7.9999 E1 0. -7.9999 7.7066 7.0000 E2 7.7066 -7.0000 16.3256 0. A1 2 16.3259 0. A1 1 24.5807 4.9988 E3 24.5807 -4.9988 31.7344 3.9967 E4 31.7344 -3.9967 37.3103 0. A2 1 37.5407 0. A2 2 41.5094 1.9952 E5 41.5094 -1.9952 43.9529 0.9973 E6 43.9529 -0.9973 44.7653 0. A3 1 −8 −6 −4 −2 0 2 4 6 8 0 10 20 30 40 hJzi Energy (meV)
Figure 4.2.: Splitting of the 4f7_{{}2 four particle state (J “ 8) of a single holmium atom
on a platinum (111) surface according to the crystal field. The colours identify the different irreducible representations of C3v (blue ” A1, red
” A2, green ” E).
can be expected. This idea was proved within the experiment, where a lifetime of τ _{“ p729 ˘ 12q s was measured [Ge6]. Thus, it is possible to magnetize a } single-holmium atom e.g. with a magnetic moment out of plane, which is related to the storage of one bit. Due to the long lifetime, this information will last for some minutes. Therefore, a single holmium atom on a platinum (111) surface can be seen as a single-bit data storage device.
Part II.
Relativistic extension of the
Korringa-Kohn-Rostoker Green
function method
5. Dirac equation and Green function
5.1. Dirac equation
With the formulation of the Schr¨odinger equation in 1926 [116, 117, 118, 119], a basic equation for the description of non-relativistic quantum systems was found. Nevertheless, the Schr¨odinger equation is not suitable for the description of elec-trons in heavy elements and furthermore for the description of spin and spin-orbit coupling. A differential equation for the investigation of electrons in relativistic quantum systems (including spin-orbit coupling) was proposed by Dirac in 1928 [120], i~B BtΨpr, tq “ ´ c ˜α¨ ˆπ ` ˜βmc2` v pr, tq ¯ Ψpr, tq . (5.1)
The vector operator ˆπ “ ˆp ´ eA pr, tq is the commonly used combination of the momentum operator ˆp _{“ ´i~∇ and the vector potential A pr, tq. The operator}
ˆ
H“
´
c ˜α¨ ˆπ ` ˜βmc2` v pr, tq ¯
is called Hamilton operator, the potential vpr, tq is the scalar potential and the abbreviations c and ~ denote the speed of light as well as the Planck constant. Furthermore, the pseudo-vector ˜αconsists of the matrices ˜αi,
which will be explained later within this section. For stationary problems, Apr, tq “ Aprq and v pr, tq “ v prq, the solution of the Dirac equation can be written as Ψpr, tq “ e´i
~W tφprq. The four component spinor function φ prq can be found by
solving the stationary Dirac equation
W φprq “ ´
c ˜α¨ ˆπ ` ˜βmc2` v prq ¯
φprq . (5.2)
The problems investigated within this thesis are stationary, and hence the term Dirac equation will be used for equation (5.2) in the following. For a classical free particle (A_{prq “ 0 and v prq “ 0), the relativistic energy-momentum relation holds,} which is given by
W2 “ c2p2` m2c4. (5.3)
In analogy to classical relativistic mechanics, equation (5.3) can be taken into account to postulate a similar relation for the free Hamilton operator,
´ c ˜α¨ ˆp ` ˜βmc2 ¯ ´ c ˜α¨ ˆp ` ˜βmc2 ¯ φprq “ W2φprq “ `c2pˆ2` m2c4˘ φprq . (5.4) 35
36 5. Dirac equation and Green function
Hence, to ensure that equation (5.4) holds, the matrices ˜α and ˜β have to fulfil the following properties, ˜ α2_{x} _{“ ˜α}2_{y} _{“˜α}_{z}2_{“ ˜β}2_{“ ˜I,} (5.5) ˜ β ˜α` ˜α ˜β “ 0, (5.6) and ˜ αiα˜j` ˜αjα˜i“ 0 i‰ j. (5.7)
These relations are satisfied by the commonly used representation [106, p. 15]
˜ αi “ ˆ 0 σ˜i ˜ σi 0 ˙ and β˜“ ˆ _{˜} I2 0 0 ´˜I2 ˙ , (5.8)
where ˜σi are the well known Pauli matrices
˜ σx“ ˆ 0 1 1 0 ˙ , σ˜y “ ˆ 0 ´i i 0 ˙ , σ˜z“ ˆ 1 0 0 ´1 ˙ , (5.9)
and ˜I2the 2-dimensional identity matrix. In general, the representation of the
matri-ces ˜αi and ˜β is not unique. Famous alternatives are given by the approach of Weyl
for massless particles [121], which is important for the description of the weak inter-action, or by the approach of Majorana, for particles without charge [122, 123]. The approach of Majorana has gained a lot of attention in recent years due to investigations of Majorana fermions in superconductors [124, 125, 126].
The solution φprq is a complex 4 ˆ 1 column matrix. Since the absolute square of the solution can be identified as the probability density of the Dirac particle, φ has to satisfy the condition
hφ|φi “ ż R3 d3_{r}_{rφ prqs}:_{φ} prq “ ż R3 d3_{r} 4 ÿ i“1 rφiprqs˚φiprq ! “ 1. (5.10)
The scalar product hφ|φi of equation (5.10) induces a norm of the solution φ prq, |φ prq| “ ahφ|φi. To satisfy (5.10), each component of φ prq has to be a square integrable function. Hence, each φiprq can be seen as a vector of the space L2pR3q,
the space of the equivalence classes of the Lebesque spaceL2_{pR}3_{q (see [127, p. 17]}
or [128, pp. 25-26]). The Hilbert space H of the solution φ prq can be constructed from the direct sum of spaces L2_{pR}3_{q [129, p. 6],}
H “ L2pR3q ‘ L2pR3q ‘ L2pR3q ‘ L2pR3q. (5.11) The Hamilton operator ˆH “
´
c ˜α¨ ˆπ ` ˜βmc2` v pr, tq ¯
of equation (5.1) is a linear operator ˆH :_{Dp ˆ}H_{q Ñ H, acting on a suitable domain Dp ˆ}H_{q Ă H. The inverse of the} operator ´´ ˆH´ W
¯
is called the Green operator or the Green function, which will be introduced in the next section.
5.2. Green function 37
5.2. Green function
The introduction of the Green function is of practical importance for the KKR method. In the sense of operator algebra within a Hilbert space, the Green function ˆGpW q can be defined as the inverse of the operator´ ˆH´ W
¯
with negative sign,
´ ˆ_{H}_{´ W}¯ ˆ_{G}_{pW q “ ´ˆI.} _{(5.12)}
Suppose the Hamilton operator has a countable set of eigenfunctions |ni which form an orthonormal basis within the Hilbert space and fulfil the completeness relationř
n|ni hn| “ ˆI. It follows from the eigenvalue equation ˆH|ni “ Wn|ni that
the Hamilton operator can be written as ˆH “ ř_{n}Wn|ni hn|. Rewriting equation
(5.12) in the form ˜ ÿ n Wn|ni hn| ´ W ˆI ¸ ˆ G“ÿ n pWn´ W q |ni hn| ˆGpW q “ ´ˆI, (5.13)
it can be verified that the Green function in operator form can be represented by ˆ G_{pW q “}ÿ n |ni hn| W ´ Wn . (5.14)
Equation (5.14) is called Lehmann representation. In real space, the relativistic Green function is a 4ˆ 4-matrix-valued function of the variables r, r1 and W and equation (5.12) can be written as follows,
´ ˆ_{H}_{prq ´ W ˜I}_{4}¯ ˜_{G}_{`r, r}1_{, W}˘
“ ´δ `r ´ r1˘ _{˜}
I4, (5.15)
where ˜I4 denotes the 4-dimensional identity matrix. The Green function has the
advantage that perturbations of the Hamilton operator can be treated in an exact manner, as will be explained in 5.4. For this approach the Green function of a reference system has to be known. Therefore, the Green function of the free electron is very important and will be derived in the next section.
5.3. Relativistic free space Green function
During this section, it will be shown, that the relativistic free electron Green func-tion (vprq “ 0, A prq “ 0) can be derived from the non-relativistic Green function G0
NR [130, pp. 413], which is given by the following equation [43, p. 192],
G0_{NR}_{pr, r}1_{, E}_{q “ ´} 1 4π 2m ~2 eik|r´r1_{|} |r ´ r1|, k“ 1 ~ ? 2mE. (5.16)
38 5. Dirac equation and Green function
From the definition of the matrices ˜αi and ˜β according to equation (5.8), the square
of the relativistic Hamilton operator is given by ˆ H_{0}2 “ ´ c ˜α¨ ˆp ` ˜βmc2 ¯ ´ c ˜α¨ ˆp ` ˜βmc2 ¯ “ `c2_{p}_{ˆ}2_{` m}2_{c}4˘_{˜} I4. (5.17)
From the operator product´ ˆH0´ W ˜I4¯ ´ ˆH0` W ˜I4
¯
“ `´~2_{∇}2_{c}2_{` m}2_{c}4_{´ W}2˘_{˜} I4
it can be verified that an equation similar to the non-relativistic Schr¨odinger equation can be obtained. Hence, the following equation can be derived for the non-relativistic Green function,
1 2mc2 ´ ˆH0´ W ˜I4¯ ´ ˆH0` W ˜I4 ¯ G0_{NR}pr, r1_{, E}_{q} “ ˆ ´_{2m}~2 ∇2_{´ E} ˙ ˜ I4G0NRpr, r1, Eq “ ´δpr ´ r1q˜I4. (5.18)
In the above equation, the energy E is an abbreviation for
E _{“} W
2_{´ m}2_{c}4
2mc2 . (5.19)
From equation (5.18) it can be seen (in comparison to (5.15)) that the relativistic Green function for a free electron is given by
˜ G0`r, r1, W ˘ “ _{2mc}1 2´ ˆH0` W ˜I4 ¯ G0_{NR}pr, r1_{, E}_{q.} _{(5.20)}
5.4. The Dyson and Lippmann-Schwinger equation
A great advantage of Green function methods is given by the fact that perturbations can be treated using the Dyson and the Lippmann-Schwinger equation [43, pp. 31-38]. A short derivation of both equations will be given within this section. The approach is valid for the non-relativistic case as well as for the relativistic case. For brevity, all equations during this section are written in operator form.
Suppose the Green function of a reference system with Hamilton operator ˆH0
is known,
´ ˆ_{H}_{0}_{´ W}¯ ˆ_{G}_{0} _{“ ´ˆI.} _{(5.21)}
Let ∆V be a small perturbation then the perturbed Hamiltonian is given by ˆH _{“} ˆ
H0` ∆V . By taking the definition of the Green function ˆG in equation (5.12)
together with (5.21), the following relation can be derived,
5.4. The Dyson and Lippmann-Schwinger equation 39
Rearranging equation (5.22) gives the so-called Dyson equation, ˆ
G“ ˆG0` ˆG0∆V ˆG. (5.23)
The Dyson equation is an implicit equation for the operator ˆG that can be solved self-consistently via ˆG _{“ ˆ}G0 ` ˆG0∆V ˆG0` ˆG0∆V ˆG0∆V ˆG0` . . . . By introducing
the scattering path operator ˆT “ ∆V ` ∆V ˆG0∆V ` . . . , equation (5.23) can be
rewritten as an explicit operator equation, ˆ
G“ ˆG0` ˆG0T ˆˆG0. (5.24)
In the next step it will be shown, how an approximation for the perturbed wave function can be found. It is assumed, that a solution φ_{0} for the unperturbed system is known, which fulfils the equation´ ˆH0´ W
¯
φ_{0} “ 0. The solution of the perturbed system φ can be constructed from the unperturbed solution via,
φ“ φ_{0}` δφ. (5.25)
Using the definition ˆG0“ ´´ ˆH0´ W
¯´1
and the eigenvalue equation
´ ˆ_{H}_{0}_{´ W ` ∆V}¯
φ“ 0, (5.26)
the following relation can be found, ´ ˆ_{H}_{0}_{´ W ` ∆V}¯
pφ0` δφq “ ∆V φ ´ ˆG´10 δφ“ 0. (5.27)
With the help of equation (5.27) the so-called Lippmann-Schwinger equation can be formulated,
φ“ φ_{0}` ˆG0∆V φ. (5.28)
The Lippmann-Schwinger equation is often used to solve the full-potential single-site scattering problem by taking into account the solution of the spherically sym-metric problem as φ_{0} and treating the non-spherical parts of the potential as a perturbation ∆V [7, 30]. From this approach it is possible to construct a set of integral equations, which can be solved iteratively, via
φ“ φ_{0}` ˆG0∆V φ0` ˆG0∆V ˆG0∆V φ0` ˆG0∆V ˆG0∆V ˆG0∆V φ0` . . . . (5.29)
The iterative solution of the Lippmann-Schwinger equation is also known as Born-series.